# Phase Transitions and Mechanical Properties of Octahydro-1,3,5,7-tetranitro-1,3,5,7-tetrazocine in Different Crystal Phases by Molecular Dynamics Simulation

Post on 23-Feb-2017

213 views

Embed Size (px)

TRANSCRIPT

Phase Transitions and Mechanical Properties of Octahydro-1,3,5,7-tetranitro-1,3,5,7-tetrazocine in Different Crystal Phases by Molecular DynamicsSimulation

Hong-Ling Cui,, Guang-Fu Ji,*,, Xiang-Rong Chen,*,,| Qing-Ming Zhang, Dong-Qing Wei,, and Feng Zhao

Institute of Atomic and Molecular Physics, Sichuan University, Chengdu 610064, China, National Key Laboratory of ShockWave and Detonation Physics, Institute of Fluid Physics, Chinese Academy of Engineering Physics, Mianyang 621900, China,State Key Laboratory of Explosion Science and Technology, Beijing Institute of Technology, Beijing 100081, China,International Centre for Materials Physics, Chinese Academy of Sciences, Shenyang 110016, China, and College of Life Scienceand Biotechnology, Shanghai Jiaotong University, Shanghai 200240, Shanghai, China

The phase transitions and mechanical properties of the energetic material octahydro-1,3,5,7-tetranitro-1,3,5,7-tetrazocine (HMX) in three pure polymorphs crystals, R-, -, and -phases, have been studied theoretically.Isothermal-isobaric molecular dynamics (MD) simulations were performed in the temperature range of (5to 555) K at 0 GPa and the pressure range of (0 to 40) GPa at 298 K. The lattice parameters and volumesshow nonlinear dependence on the temperature and pressure. In the high-temperature regime, there existtwo phase transitions, that is, from - to R-HMX at 360 K and from R- to -HMX at 440 K. Under highpressure, the -HMX transition to -HMX is shown at 27 GPa and 298 K. Within the range of temperatureand pressure studies, it can be deduced that the -HMX at lower temperatures and higher pressures, theR-HMX at higher pressures, and the -HMX at lower temperatures have better malleability.

Introduction

As we all know, HMX1 (octahydro-1,3,5,7-tetranitro-1,3,5,7-tetrazocine) has been an important and useful energetic materialas a secondary explosive since the 1930s. There exhibits fourdifferent crystal structures of HMX, three pure crystallizationphases, R, , and , and a hydrate phase .2 At ambientconditions, the stabilities of these polymorphs are known to be > R > > .3 The -HMX phase, with the monoclinic P21/cspace group, is the most stable form.4 It has the highest energyand density and the lowest sensitivity at ambient conditions.4

The crystalline phase has been investigated to contain twoC4H8N8O8 groups, and the symmetry axis is b, thirteenindependent elastic coefficients by X-ray and neutron diffraction.5,6

The R-HMX phase has been studied to contain eight C4H8N8O8groups, with the orthorhombic Fdd2 space group and nine elasticindependent coefficients.5 The -HMX phase is formed at thesolid-melt interphase in deflagrating HMX, has a hexagonalP6122 structure, c symmetry axis, and five independent elasticcoefficients, and is considered to be stable at extreme conditions.7,8

The -HMX phase has been investigated to contain twoC4H8N8O8 0.5H2O molecules per unit cell, with the Pn sym-metry space group.4 Cady and Smith observed two phasetransitions; that is, one is the - to R-HMX transition at (375 to377) K, and the other is the solid R- to -HMX transformationat (433 to 437) K.2 Yoo and Cynn9 found two phase transitionsby the diamond-anvil cell, using angle-resolved synchrotronX-ray diffraction and micro-Raman spectroscopy; one is theconformational change at 12 GPa with no apparent volume

change, and the other is the phase transformation along with a4 % volume discontinuity at 27 GPa. Gump and Peiris10 andStevens and Eckhardt11 have studied the compression of -HMXby synchrotron angle-dispersive X-ray diffraction techniques andscattering from a variety of acoustic phonons, respectively.Computational studies were carried out to investigate theinfluence on the lattice parameters at different pressures ortemperatures of -HMX.1216 The energetic stabilities andvibrational properties of HMX were simulated by using firstprinciples at different conditions.1721

Despite the above efforts, the phase transition and mechanicalproperties of three pure polymorphs of HMX crystal have notbeen explored completely, especially at high pressures and hightemperatures. These properties are important to understand HMXcrystals. In this work, we carried out molecular dynamics (MD)simulations to study the phase transition and mechanicalproperties of pure HMX crystals under different temperaturesand pressures.

Computational Methods

In this paper the MD simulations were performed with theDISCOVER module of the commercial software MaterialsStudio.22 The COMPASS (condensed-phase optimized molec-ular potentials for atomistic simulation studies) force field23 wasused with a cutoff distance of 10.5 . The MD simulations werecarried out in the normal pressure and temperature (NPT)ensemble with the Berendsen barostat method24 and Andersenthermostat method25 to control the system pressures andtemperatures. The simulation supercell contains 96 HMXmolecules and 2688 atoms, corresponding to the boxes of 4 4 3, 3 2 2, and 4 2 2 unit cells for the -HMX,R-HMX, and -HMX, respectively. The initial crystal latticeand atomic position of -HMX, R-HMX, and -HMX weretaken from the experimental results of refs 9, 5, and 8,respectively. The long-range nonbond Coulombic and van der

* To whom correspondence should be addressed. Tel.: +86 816 2485108;e-mail address: cyfjkf@caep.ac.cn (G.-F.J.). Tel.: +86 28 85405516; e-mailaddress: xrchen@126.com (X.-R.C.). Sichuan University. Chinese Academy of Engineering Physics. Beijing Institute of Technology.| Chinese Academy of Sciences. Shanghai Jiaotong University.

J. Chem. Eng. Data 2010, 55, 31213129 3121

10.1021/je100009m 2010 American Chemical SocietyPublished on Web 03/30/2010

Waals interactions were managed using the atom-based sum-mation method.26 A fixed time step of 1 fs was used in all MDsimulations. At each temperature and pressure, the system wasfirst relaxed for 1 105 time steps in the equilibration run,followed by a production run of 1 105 time steps. The data fromthe production run were collected for subsequent analysis.

Results and Discussion

Choice of Force Field and Equilibrium of System. Figure1 displays the supercell models of the crystalline R-, -, and-HMX in the initial MD simulation. To choose a suitable forcefield, we carried out a series of tests for -HMX, R-HMX, and-HMX crystals. The parameters of the COMPASS force fieldhave been tested and confirmed by comparing with theexperimental values. The nonbond parameters have been furthermodified by the thermal physical properties of liquid and solidmolecules obtained from the MD method. In previous studies,the COMPASS force field was employed in the MD simulationsof many nitramine explosives, such as bicycle-HMX, CL-20,and TNAD.2731 The results of MD calculated are listed in Table1. The discrepancy between our results and the experimentalresults is small, that is, 0.61 %, 0.63 %, 0.69 %, 2.01 %, and1.97 % of a, b, c, V, and F for -HMX, 1.12 %, 1.17 %, 1.18%, 3.54 %, and 3.4 % of a, b, c, V, and F for R-HMX, 0.65 %of a, b, and c, 1.92 % of V, and 1.88 % of F for -HMX,respectively. The simulated results of geometry parameters arein good agreement with the experiment, indicating that theCOMPASS force field is appropriate for simulating the HMXcrystal.

Before the statistic analysis, the system must reach theequilibrium state. The equilibrium of the system is achievedwhen the fluctuations of temperature and the energy are lessthan 10 %. Typically, the system should achieve its equilibriumin the initial 100 ps, followed by a production run of latter 1 105

time steps. It can be seen that the system temperature hasreached its equilibrium state within (288 to 308) K (298 ( 10K) from our results. The amplitudes of fluctuations for potential

Figure 1. Initial supercell models of HMX in the MD simulation. The left is -HMX supercell model, the middle is the R-HMX supercell model, and theright is the -HMX supercell model.

Table 1. Lattice Parameters Simulated by the COMPASS ForceField Compared with Experimental Values of r, , -HMX at 298 Kand 1.0 10-5GPa

a b c R V F

deg 3 g cm-3

-HMX ref 9 6.54 11.05 8.70 90 124.3 90 259.7 1.89this work 6.58 11.12 8.76 90 124.3 90 264.9 1.86

R-HMX ref 5 15.14 23.89 5.91 90 90 90 267.2 1.84this work 15.31 24.17 5.98 90 90 90 276.6 1.78

-HMX ref 8 7.71 7.71 32.55 90 90 120 279.4 1.76this work 7.76 7.76 32.76 90 90 120 284.7 1.73

Figure 2. Lattice parameters of -HMX at different temperatures, 0 GPa, inthis work and atmospheric pressure in ref 15. 9, a in this work, 0, a in ref 15;b, b in this work; O, b in ref 15; 2, c in this work; 4, c in ref 15.

Figure 3. Lattice parameters of R-HMX at different temperatures, 0 GPa,in this paper and atmospheric pressure in ref 15. 9, a in this work; 0, a inref 15; b, b in this work, O, b in ref 15; 2, c in this work, 4, c in ref 15.

3122 Journal of Chemical & Engineering Data, Vol. 55, No. 9, 2010

energy and nonbond energy are less than 0.3 % and 0.2 %,respectively, showing that the system has reached its energyequilibrium. After equilibration, production runs of 100 ps werethen performed.

Phase Transition under Different Temperatures andPressures. Within NPT ensembles, we calculated the structuralproperties and phase transition of the -, R-, and -HMX atdifferent temperatures and 0 GPa and at different pressures and298 K. We simulated the structural properties in the range of(5 to 400) K at 0 GPa and the pressure range of (0 to 31) GPaat 298 K for -HMX, in the range of (350 to 480) K at 0 GPaand the pressure range of (22 to 40) GPa at 298 K for R-HMX,and in the range of (430 to 555) K at 0 GPa and the pressurerange of (20 to 40) GPa at 298 K for -HMX.

Under Different Temperatures. Under different temperatures,the lattice parameters and volumes are listed in the Figures 2to 5 together with the results of ref 15. The lattice parametersand volumes vary nonlinearly with temperature and exhibit an

abrupt change at 360 K in the temperature range (5 to 400) Kfor -HMX, at (380 and 440) K for R-HMX, and at 440 K for-HMX. From Figures 2 to 5, we found two phase transitions:one from -HMX to R-HMX at (360 to 380) K agrees with theexperimental result at (375 to 377) K,2 and the other fromR-HMX to -HMX at 440 K agrees with the experimentalobservation of the phase transition at (433 to 437) K.2 Withtemperature increasing the lattice parameters and cell volumesincrease, and the crystalline density of three phase decreasesgradually in their stable temperature ranges. In the temperaturerange of (5 to 350) K, the ratio of the change of a, b, c, and Vare 2.31 %, 2.37 %, 2.44 %, and 7.35 % for -HMX. Withinthe range of (380 to 440) K, for R-HMX the changes of latticeparameters are 0.73 %, 0.74 %, and 0.88 % for a, b, and c,respectively; the cell volume change is 2.2 %. For -HMX, withtemperature increasing from (440 to 555) K, the latticeparameters increase in 0.91 % for a, b, and c, and the cellvolume change is 2.7 %. In the corresponding temperature range,the change trend of the lattice parameters and cell volume ofour results agree with Sorescu et al.15 The reason of thediscrepancy for -HMX is that the initial structure is different;the space groups are P21/c in our work and P21/n for Sorescuet al. Moreover, our results agree with the experimental resultswell. While, within the entire temperature range considered, thelattice angles almost remain invariant, that is, R and areapproximately equal to 90 and remains approximately 124.3for -HMX, R ) ) ) 90 for R-HMX, and R ) ) 90and ) 120 for -HMX, respectively.

The thermal expansion coefficient is an important parameterto characterize the physical and the explosive behavior of theenergetic materials. The linear and volume coefficients of-HMX, R-HMX, and -HMX are listed in the Table 2. Theaverage linear coefficients of -HMX, 6.884 10-5 K-1, agreewith the previous experimental result of 5.04 10-5 K-1.32 Thereexits a small discrepancy between our results and ref 15 for thedifferent temperature range and space group possibly. Figures2 to 4 show that the thermal expansion of the -HMX andR-HMX is weakly anisotropic. Expansions along the crystal axesb and c are 2.37 % and 2.44 %, respectively; both are slightly

Figure 4. Lattice parameters of -HMX at different temperatures, 0 GPa,in this work and atmospheric pressure in ref 15. 9, a in this work; 2, a inref 15; O, b in this work, 3, b in ref 15; f, c in this work, g, c in ref 15.

Figure 5. Unit cell volume V as a function of temperature for three HMX, 0 GPa, in this work and atmospheric pressure in ref 15. 9, this work (-HMX);0, ref 15 (-HMX); 2, this work (R-HMX); 4, ref 15 (R-HMX); b, this work (-HMX), O, ref 15 (-HMX).

Journal of Chemical & Engineering Data, Vol. 55, No. 9, 2010 3123

larger than that along the a-axis (2.31 %) in the temperaturerange of (5 to 350) K for -HMX. Furthermore, we found thatboth linear and volume thermal expansions of the three phasesvary slightly with the temperature increasing in their stabletemperature range, but the temperature effect on the thermalexpansion can be nearly ignored due to the very small amplitude.

Under Different Pressures. Under different pressures, thelattice parameters and volumes under different temperatures arelisted in the Figures 6 to 9 for -HMX, -HMX, and R-HMX.From Figures 6 and 9, the lattice parameters and volumes of-HMX vary nonlinearly with pressure and exhibit an abruptchange at 27 GPa in the pressure range (0 to 31) GPa, whichagrees with the results of Yoo and Cynn.9 From Figures 7 and

9, R-HMX phase exhibits two abrupt changes: at (25 and 38)GPa. From Figures 8 and 9, we found that the -HMX phaseundergoes two abrupt changes: at (25 and 36) GPa. That is tosay, R-HMX and -HMX phases are relatively stable in thepressure range of (25 to 38) GPa and (25 to 36) GPa,respectively. It indicates that -HMX undergoes a phasetransition at 27 GPa, in agreement with the experimental9 andtheoretical16 results. While -HMX will transit to the R-HMXphase or the -HMX phase, it depends on the stability ofR-HMX and -HMX phases under high pressure. We canestimate it from the total energy of R-HMX and -HMX phasesin the range of the (25 to 36) GPa. Figure 10 shows that thetotal energy of -HMX phases is lower than that of the R-HMXphase, that is, the -HMX phase is the stable phase in the rangeof (25 to 36) GPa until it can be detonated over 36 GPa, whichagrees with the explosive pressure of 39 GPa.32 Hence, -HMXexhibits a phase transition to the -HMX phases at (25 to 27)GPa. With pressure increasing from (0 to 27) GPa, the latticeparameters and cell volumes decrease, and the crystalline densityof -HMX increases gradually. In the pressure range of (0 to27) GPa, the ratios of the change of lattice parameters andvolumes are 14.4 %, 14.3 %, 15.6 %, and 37.1 % for a, b, c,and V, respectively. The ratio of the compression of latticeparameters and volumes of -HMX phases are 2.45 % and 7.16% for a, b, c, and V, respectively. The ratio of compression of-HMX agrees with the experimental resul...

Recommended